Iowa State University Capstones, Theses and Retrospective Theses and Dissertations Dissertations
1968 Optical properties of halides of silver and thallium under hydrostatic pressure Alfred Douglas Brothers Iowa State University
Follow this and additional works at: https://lib.dr.iastate.edu/rtd Part of the Condensed Matter Physics Commons
Recommended Citation Brothers, Alfred Douglas, "Optical properties of halides of silver and thallium under hydrostatic pressure " (1968). Retrospective Theses and Dissertations. 3649. https://lib.dr.iastate.edu/rtd/3649
This Dissertation is brought to you for free and open access by the Iowa State University Capstones, Theses and Dissertations at Iowa State University Digital Repository. It has been accepted for inclusion in Retrospective Theses and Dissertations by an authorized administrator of Iowa State University Digital Repository. For more information, please contact [email protected] This dissertation has been microfilmed exactly as received 68-14,774 BROTHERS, Alfred Douglas, 1939- OPTICAL PROPERTIES OF HALEDES OF SILVER AND THALLIUM UNDER HYDROSTATIC PRESSURE.
Iowa State University, Ph.D., 1968 Physics, solid state
University Microfilms, Inc., Ann Arbor, Michigan OPTICAL PROPERTIES OP HALIDES OP SILVER AND THALLIUM
Umza HYDROSTATIC PRESSURE
Alfred Douglas Brothers
A Dissertation Subraitted to the
Graduate Faculty in Partial Fulfillment of
The Requirements for the Degree of
DOCTOR 0? PHILOSOPHY
Major Subjects: Physics Education
Signature was redacted for privacy. In Charge of i- ^or Work
Signature was redacted for privacy.
Heads oM iajor Dep rtments
Signature was redacted for privacy. att of Grad te College
Iowa State University Ames, lo^a
TABLE 0? CONTENTS
Pa,3e INTiiODUCTIOM 1 APPARATUS 12 EXPERIMENTAL 20 RESULTS 31
DISCUSSION 52 SUMi'IAHY AND CONCLUSIONS ?1
LITERATURE CITED 74
ACKNOWLEDGEMENTS ?? INTHOIWCTIO:';
The use of hydrostatic pressure, combined v.'lth lovf tem peratures, is a valuable technique In the study of crystal properties. Pressure changes the lattice parameter while leaving the vibrational amplitudes of the ions essentially unch^n^ed. This may be contrasted to the effects of chanjln^ the temperature of the sample, which alters both the lattice parameter and the vibrational anplitude;: of the ions. At lov; temperatures only the lov.'est vibrational states of the crystal are excited. This results ezperlaenûally in a better resolved and simpler optical spectrum. In this work the effects of hydrostatic pressure applied to sin.,.;lc crystals and thin evaporated films of A:r3r, Aj^^CI, TlBr, and TlCl were studied optically at low temperatures. As is well knoim, insulators have an energy gap, Eg, of a few electron volts (eV) between their valence and conduction bands. Electronic transitions from the valence to the conduc tion band are stimulated by incident photons of energies near
Eg and greater. For the above four materials, this occurs in the visible to near-ultraviolet wavelength region. The shape of this absorption edge and its position with respect to Er are properties of the band structure of the crystal. The pressure shift of this absorption edge can yield information about the relative changes in the valence and conduction band structures. Similar pressure shifts for the absorption edges of crystals whose crystal structures are quite similar, which
will be shown to be the case for A.'/Sr and AgCl, indicate elec tronic transitions from valence bands of the same symmetry to conduction bands of the same symmetry. At incident photon energies generally below those at the
beginning of the absorption edge lia absorption peaks caused by the formation of excitons. Excitons may be defined as quanta of non-conducting electronic excitation energy asso
ciated with the entire crystal, whoae motion through the •
periodic crystal lattice may be characterized by a wave vec tor. They may alternately be thought of as a loosely bound electron-hole pair with effective masses £,nd respec tively, separated by a dielectric medium. This describes the very useful Wannier exciton model (1). Discrete exciton ener,.';y levoln exint immediately below the conduction b^nu.
These discrete levels may produce a series of exciton absorp tion peaks near or superimposed upon the absorption edge.
Thin evaporated films of Ag3r, AgCl, TlBr, and TlCl were studied since the exciton absorption peaks occur at much higher levels of absorption than could be measured using thick single crystals. In these films the absorption in the wavelength region of the exciton peaks was sufficiently low so that the desired optical measurements could be made.
There exist several possibilities for the shape and posi tion of the absorption edge, each of which implies a differen 3
exciton absorption spectrum. The momentum which the incoming photons supply to the crystal is negligible compared to the
momentum of a typical electron in a crystal. For the case in
which the valence band maximum appears directly below zhe con
duction band minimum, the transition is called a direct trans
ition. An electron is raised from the valence band to the
conduction band with no change in momentum (or wave vector k).
See Figure la. The onset of absorption is depicted by transition 1
between the two cxtronn. Thlr oocurn at the enor>';y, li,.-.
As the transitions occur farther away from the maximum of the valence band, as transitions 2 and 3 in Figure la, increasing
ly greater numbers of electronic states are involved, result
ing in the increase of the absorption coefficient,#, as shown
in Figure lb. The shape of the absorption edge varies as
("hcv -2g)2 (2) where iiCJ is the incident photon energy. The discrete states arising from the creation of excitons have binding energies, B, of a few hundredths of an eV as
measured from the conduction band. Since incoming photons
provide essentially no momentum for the electron-hole pairs they create, the transitions are all essentially vertical.
Excitons can have net momenta and kinetic energy of motion through the lattice, described by exciton energy bands, shaped similarly to the conduction band, which appear in Figure Ic. Only the states of zero momentum can be reached by absorbing a 4
DIRECT EDGE NO ELECTRON-HOLE INTERACTION
En b \\v
WITH ELECTRON-HOLE INTERACTION
-> E d h V
Fleure 1. Schematic representation of the direct absorption edge 5 photon, however. Transitions fron the valence band maxiEui to these levels (A, C, and D in Figure Ic) result in the nodified spectrum of the edge as displayed in Figure Id. Using the
Wannier model, the oscillator strengths of the peaks corres ponding to transitions A, C, and D vary as n~5 where n = 1 represents the lowest discrete energy level, and the oscil lator strength of a band may be defined as the integrated area under the absorption band. For this reason often only the absorption peak corresponding to the n = 1 transition is seen experinontally. The enhancement of the absorption beginning at i2,. is due to the creation of electron-hole pairs v/hich remain nearby, since the incident photons here cannot supply energy enough to separate the electron and hole rapidly. This condition increases the value of the matrix elements which determine the intensity of absorption. As the energy in excess of that needed to create the free electron and hole increases, that is, the incident photons become more energetic, this enhance ment decreases. The indirect edge is treated schematically in Figure 2.
Here the conduction band minimum and the valence band maifimum lie at different values of k. Transition 1 (Figure 2a) occurs with the absorption or emission of a phonon to conserve momen tum. The possibility of transitions which absorb or emit phonons adds to the complexity of the indirect absorption 6
INDIRECT EDGE NO ELECTRON-HOLE INTERACTION J
WITH ELECTRON-HOLE INTERACTION
c ! I I I
_l£ L ig-k^B Eg-kg (j hi/
Figure 2. Schercatic representation of the indirect absorp tion cd^-e 7
edge. The beginning of the absorption edge is at (Eg-kQ),
where kG represents a phonon energy of typically a fev: hun dredths of an eV. Transitions such as 2 and 3 also occur, utilizing phonons of different aoatnta than'transition 1.
The increase in the number of states farther from the valence band maximum again produces the rise in absorption vrith increasing incident photon energies. Notice that the func tional dependence of the edge here is (nw -Eg + kO)^ (2) com pared with (hW"2j)- for the direct edge. This suggests that the indirect edge should rise more sharply than the direct edge. The fact that the opposite condition is generally seen points out the importance of the coefficients of these terms, which are not included here.
Introduction of electron-hole interactions again compli cates the absorption spectrum. Transitions A and D (Figure
2c) differ not only in the energy change vhlch they effect, but also in the momentum of the phonon needed for the transi tion. Prom this it can be seen that a broad range of energies is available for transitions to each exclton energy level. Thus the added absorption component, beginning now at (E^-kO -B), is devoid of sharp peaks (Figure 2d). Another cause of this structureless absorption is that two transitions may occur from the same location on the valence band, yet proceed to different k values on the exciton energy bands. This could create two excitons of similar energies, but very different momenta, just aa transitions A and C croate two excitons- of comparable momenta but quite different energies. For either the direct or Indirect transitions both allowed and forbidden transitions can occur. Allowed and forbidden are used here in a sense siiailar to allowed and forbidden transitions in the hydrogen atom problem, governed by angular momentum selection rules.
It should be noted that although the oscillator strengths for excitons are only about 0.1 as compared to 0.8 or better for many defects in a crystal lattice, the exciton absorption peaks can be quite prominent. This is possible because every atom in a crystal is capable of yielding an exciton,.compared to perhaps one in ten thousand or more for defects or impuri ties.
Table 1 (2) contains a suimnary of the expected functional dependence of the absorption edge and the exciton spectra for all the above-mentioned cases.
Although exciton absorption peaks generally occur at energies below Eg, germanium offers an example of a system in which this absorption occurs at energies greater than 2^ (2).
The lower energy absorption edge in germanium is an indirect edge at about 0.6 eV. A second edge appears at about 0.8 eV.
Associated with this edge is a direct exciton, which, as a result, appears about 0.2 eV above the onset of absorption.
A further complication in the spectra studied in this 9
Table 1. Summary of the functional dependence of the absorp tion edge and excitons for direct and indirect transitions icrgy dspciiicncô of optical absorption cocuicicnt k
Transition Exciton CUCCtG IZ.'iciion included nci'Icctcd
Lines at R hcû — "J rt ~ ii 2f jf 4t, n'
Dircc; allowed For the co:.iiav.Mza —icxp -« ^ v/ncrii a - Sinn 7:a
,ncs fico-Eo-~, « = 2,3,4... n n^ — 1 Â- Dircct forbidden i For the continiiuiii A . l\ expr:ci !\ - T ay— —n—sinh na
(nco-£J±1CÛ)^ M = 1,2, 3. Indirect allowed components For the continuiir.i
^wuna excitons O'i(o-ji:^±kûf ;r-i. (/iw-;:'±Z:0)^ /; = 2, 3, fr.Jircct fbirbidilcu conioonents ror uie continuua 10 work arises from the large number of electrons available from both the anions and cations of the four crystals studied.
Band structures resulting from so many electrons cannot be expected to be either simple or isotropic in k space. Appli cation of pressure will likely cause a non-uniform distortion of these band structures. Paul (3) has found that different band edges likely have different deformation potentials, which makes pressure experiments valuable in sorting out complicated band structures^ The deformation potential may be defined as
when hydrostatic pressures are used. He also suggested that changes in position and shape of the optical absorption edge can be clues to the presence of different scattering mechan isms, particularly impurity scattering, and of multiple extrema having different pressure coefficients.
The present work was undertaken as an attempt to under stand better the band structure of the silver and thallium salts studied. The silver salts have been extensively studied, and calculated band structures which exhibit the known charac teristics of the absorption edges and excitons in these salts are available and in general agreement (4,5). Because of the complexity of the silver salt band structures, to be discussed later, the added information obtained here is valuable in sorting out some areas of important, albeit subtle, disagree- 11 ment in the calculations. Although no similar calculations have been attempted for the thallium salts, several other recent experiments have provided insights into their band sti'uotures. APPARATUS
The pressure generating system (see Figure 5 for a block diasram) was designed to attain pressures up to 10,000 atmospheres using helium gas as the pressure transmitting fluid. The system was charged with helium gas from an auxil iary pressure system which boosted the pressure to about 350 atmospheres from 150 atmospheres out of the tank. This system was then valved off and the pressure regulated as desired with the main system. Because of the reduced dimensions of tne pressure cell used in this experiment, a pressure of 3500 atmospheres was judged to be the maximum safe pressure. This limit did not impose severe restrictions on the accuracy of the pressure shifts measured, since most were large even over the limited range available. Thus the intensifier (I Figure
3) and related parts were not used. The pressure system employed a Southern California Engi neering Corporation air driven oil pump capable of producing oil pressures to 4^00 atmospheres. This pump was used to drive the piston of the oil-helium separator (S Figure 3). The separator vras machined from Allogheny-Ludlum Almar 300
tccl lind provided v;it;h a proui^ci.lvc iron xhciLli pressed over its length. The pressure sealing rings were of standard design, composed of neoprene and lead washers sand wiched between discs of maraging steel and forced against a polished seat by the retaining nuts. The location of the Figure 3. Block diagram of pressure system used in the experiment F ~ Air filter and oiler P " 0"70f000 psi hydraulic puiup R - Oil reservoir and filter 3x~ Oil bleed valve Gi" 0-75,000 psi Bourdon gauge (oil) S " Oil-helium separator I •» i]arv:ood A2.5J intensifier V - 200,000 psi needle valve T '• Oil trap K " Kanganin gauge Bg- Helium bleed valve G2" 0-7000 psi Bourdon gauge (heliu.ri) indicates l/'J" O.D. >: OcOoO" I.D. stainless steel tubing indicates 1/16 " O.D. x 0 « 020" I.D, stainless steel tubing indicates 1/0'' O.D, x 0.020" I,D. stainless steel tubing I
D2 ^ s" TO HELIU!/, TANK
X) V I"'-p-
IUi.H 1- ' ™ ''2_CEL'. 15 piston in the separator was monitored using a linear variable differential transformer mounted over a length of 3/8" diam eter pressure tubing. Inside the tubing rode a soft iron slu^ attached by a long non-magnetic rod to the piston, A balanc ing circuit driven by a servo motor connected to the trans former by a cord kept the transformer centered about the core.
The position of the piston could then be determined by the position of a pointer on the servo motor shaft.
Pressure tubing used v:as 1/8" diameter 60,000 psi test and 3/16" diameter, both ifith a 0.020" hole. Tubing contain ing the helium gas was 100,000 psi test stainless steel. The oil lines were 1/4" diameter 60,000 psi test stainless steel. All valves used were 60.000 psi test. As a safety precaution the system was enclosed in a I/o" steel-plated cart. The design of the pressure cell (see ?i,gure 4) was a result of several preliminary test models (6) and proved very satisfactory. Made also of maraglng steel, it measured 2 5/5" in diameter by 2" high. The sealing surface of the cell body was carefully polished before and after hardening the steel.
The "mushroom" plugs (R) are of the unsupported area design
(7) and also made of maraging steel. The surfaces onto which the sapphire windows were attached were machined flat, then polished in a vibrating bed polisher with alumina until they appeared smooth when viewed under a microscope. The sapphire windows, oriented with the c-axis perpendicular to the flat Figure H-. Pressure cell C - Cell body S - Sample holder N - Retaining nut B " Brass extrueion ring R Pressure seal I - Indium gasket W - Sapphire window A - Steel retaining ring 17 face and flat to vrlthin 0.0001", were varnished onto the mushroon plugs with General Electric 7031 low temperature varnish. The brass extrusion rings (3) were of triangular cross section and served to prevent the indiuia sealing ring (I) froa extruding and jamming the plus i:n the cell. The hex-head maraging steel nuts (N) were tightened securely against the retaining ring (A). The optical path was a cone of 10° included angle, with minimum openings of 3/l6" at the sapphire window seats.
The cryostat used was a double reservoir, single vacuum jacket container (Figure 5)» The pressure cell was bolted to the bottom of the heliun reservoir by ineans of a copper disc which was first bolted to the cell, ôhen this assembly bolted to the cryostat. Pressure was introduced into the cell through a section of the 1/6" tubing described above, running through the center of the cryostat. The tubing xcas sealed at the top with a compression type 0-ring vacuum seal, A spacer was provided to center the tubing in the shaft as well as to lengthen the distance between the portion of the tubing at liquid nitrogen temporature and that nt room temperature. The inner radiation shield was kept at the temperature of the liquid in the inner reservoir. The outer shield was held at liquid nitrogen tenperature. The quartz windows were waxed into place, since more elaborate seals were too bulky to allow the cryostat to fit into the sample chamber of the Gary 14% 18
®il I 'xr %
! t' li !i\.v ru A-.
III Jl i Jl
D' ,b I li"r- m
JTdn. SI :yy:
Figure 5»' Optical heliua cryostat used in pressure experi ments 19
spectrophotometer. The cryostat was ir.achlned fro% stainless steel, except for the outer wall which was aluminum. The cell
•and the inner reservoir were held in place by the soft solder
joints at the inner reservoir vent and fill tubes. These
joints were sufficiently sturdy uo support the several pounds
of the cell, reservoir, and shield, and regained leak tight.
The capacity of the inner reservoir was about 2 liters. The cryostat was supported on the spectrophotometer by a rigid stand mounted on the table supporting the spectrophotometer, since the assembly was too heavy to rest directly on the cantilevered sample chamber.
The cryostat used in making the temperature dependence measurements was a Cryonetics single vacuum jacketed cryostat with an exchange gas chamber surrounding the sample chamber.
Small amounts of helium exchange gas could be added or removed by a system of valves mounted on the cryostat. Temperatures were measured with a Au-0,02;^ Pe versus Cu thermocouple (8) calibrated carefully to SO°K, with the calibrations extrapo lated to 273°K. A heater was provided on the sample holder to allow regulation of the sample temperature. EXPERIMENTAL
Samples and Sample Preparation
Samples of the single crystals were obtained from various sources. The T13r and TlCl samples wore from the liar s haw
Chemical Company. Earlier samples of T13r and TlCl from Vinor Laboratories not only were colored when received, but %ave peculiar results when measured. They were therefore not used. A Vinor AgBr sample was purchased, but it too failed to re spond in a believable manner. The A^Cl sanple and a very pure zone refined AgBr sample were obtained from Dr. R. 3. Van Heyningen at the Eastman Kodak Research Laboratory. These yielded spectra which were in excellent agreement with already available results. The crystals were nominally 2 nm thick by
9 mm in diameter when ready for use. Polishing was done on a wax lap using 1 micron and 0.3 micron alumina in water, fol lowed by a few light passes over a facial tissue. The AgCl sample was annealed at 250^0 for several hours in a chlorine atmosphere to remove colloidal silver deposits present. The crystals were exposed only to light from Kodak Wratten lA filters while polishing and loading into the cryostats. The thin film samples were made from reagent grade chem icals evaporated onto quartz substrates. These substrates were carefully cleaned prior to the evaporations by first scrubbing with an alcoholic KCH solution, then rinsing with solvents and distilled water until the water covered the 21 quartz in an even layer. The substrates were then dried with a strean of hot air and loaded immediately into the evapora tor. A 25 quartz plate was placed next to the sample sub strate. The square quartz rested on a stainless steel support which masked a strip about 2 mm ifide across the center. After the evaporation this mask was removed and the whole square overcoated with a layer of silver by evaporation. These were used to make thickness measurements of the samples.
The evaporator was composad of a ?" diameter pyrex bell jar usin.3 a teflon seal, dumping was done by two 4 liter per second Varian vacion pumps after the system was roughed ou%.
Typical evaporation pressures were 10"^ Torr, with a sample to substrate path length of about 10 cm, considerably smaller than the mean free path of the evaporating molecules. Evapor ations were made as rapidly as was consistent with the above- mentioned pressure limit. To prevent spattering of the silver salts while evaporating, a closed tantalum cylinder with two small holes pointed in the general direction of the sample was used. Evaporations of the thallium salts went smoothly and rapidly directly from the tantalum boat. Due to the low evaporation temperatures of all these salts, outgassing of the sample before evaporation was not fcanl.ule.
Thlc'cnoiî;.-; muaixirenicnL: vccro initially i:;ado on a cpcc- trometer modified and calibrated by Kr. R. Horgan. Inter ference effects which arose from bringing the silver overcoated sample substrate in contact with a half silvered reference mirror provided the means of measuring the thickness (9» P.
105). Later a Varian multiple beam interferoiaeter was o obtained, whose accuracy was reported to be ^ 30 A. Checks between the modified spectrometer and the Varian interfer ometer indicated that the spectrometer was well calibrated, although somewhat less accurate than the interferometer.
Special care was again taken to prevent white li^ht from striking the films. The silver halide films clouded immedi ately on exposure to white light. The evaporator was shrouded before and after the evaporation, and the evaporation was performed in a dark-room. The films were handled under light from Kodak Wratten lA filters. The films were generally placed in the cryostat immediately after they were produced.
The crystals were studied as follows. The pressure seal ing windows were varnished onto the mushroom plu^s. After at least several hours of drying time, the excess varnish was removed from the optical path of the plug assembly. The sample was then placed in the pressure cell, this mounted in the cryostat, and the cryostat evacuated. The initial pres sure had to be about 1000 atmospheres to prevent helium leak age through the varnish seals when they were cooled. The cryostat was then cooled by placing liquid nitrogen in both reservoirs. After about three hours, the pressure was incTo.a;::od to tho (iu::1 r»xl usually aVjoat 3000 23 atmospheres. The liquid nitrogen was blovm out of •che inner reservoir and the helium transfer begun. Unfortunately there was no way to introduce a thermocouple into the saraple chamber of the pressure cell. A thermocouple attached to the copper mounting disc or to the exterior of the cell was of little value, since these areas are the first to cool. The transfer was made slowly, usually over a period of 40 minutes. This
Was done to allow the cool helium sas to cool the sample most effectively as well as to insure an ample aaount of helium in the reservoir when the transfer w&s over, since the cell took a considerable length of time to cool to an equilibrium tem perature. During the runs the vacuum pumping system, con sisting of a fore pump and an oil diffusion pump, was left connected in case a minor pressure leak might occur.
Helium solid!ficn at at elevated .
It was assumed that solidification would bc^in first at the region where the mounting plate and the pressure tubing outlet were located. If this were the case, which is most likely, the pressure in the trapped volume of the sample chamber would drop in accordance with the pressure vs. temperature diagram of solid helium (10). For pressures near 3000 atmospheres a pressure drop of 8/i upon solidification was estimated from this curve. The slight decrease in pressure upon cooling to nitrogen temperature was automatically accounted for by read ing the pressure as the helium transfer began. Judging from 24
the fact that the optical densities before and after transfer
were essentially the same, and the fact that the sample nearly fills the optical path through the sample chamber, no ill
optical effects due to the change of state of the helium were
to be expected.
The cryostat was left in place after the spectrum was
measured. After warming to near room temperature overnight,
the sample chamber was brought to room pressure. The varnish
would fail at this low pressure and the remaining helium would
enter the vacuum jacket and be removed by the pump. This
procedure,, in effect, extended the available pressure range
by 1000 atmospheres and also insured that no difficulties would appear with the pressure seals after they had been once cycled to liquid helium temperature. The pressure tubing was sealed off at the top of the cryostat to limit the volume of gas to be pumped out before recooling. After the vacuum had recovered, the same cooling procedure as above was used to run another spectrum at zero atmospheres and 10°K.
Because the absorption edges are temperature dependent and no thermocouple could be installed to assess the actual temperature of the sample, the best procedure to attain a reproducible temperature was to allow the pressure cell to come to some equilibrium temperature. Careful account was kept of the time elapsed from the beginning of the helium transfer, and this was used as another method of obtaining 25 reproducible temperatures, especially when the helium boiled away before an equilibrium temperature was thought to be reached. This problem arose only for the A3CI runs, where the spectra were taken one hour after the transfer began. For the other three salts the tizes of the measurement were three hours after the transfer began. It was felt that equi librium had been reached at those times. Since the helium usually remained for up to seven hours after transferrin.^, it was felt that not only had an equilibrium temperature been reached, but that this temperature was quite near liquid helium temperature. By comparison of the position of the TlCl crystal absorp tion edge obtained at zero atmospheres to the position of those absorption edges made for the determination of the tem perature dependence of the same TlCl single crystal, the sample temperature in the pressure cell after three hours of cooling with liquid helium could be determined to be 10°X, to the nearest degree» The procedure for measuring the pressure shifts of the peaks of the excitons in thin films was somewhat different, since these spectra were made only at liquid nitrogen tempera ture, Again the cryostat was cooled for at least three hours prior to the experiment, allowing the cell to come to an equi librium temperature. The minimum pressure used was again about 1000 atmospheres. Spectra were taken in increments of 26 about 300 atmospheres to the naxinun pressure desired, vrhich was usually about atmospheres. As a check to determine the extent of any irreversible strains, or a shift in temper ature while the experiment %ras proorcsslnç, ' spectra were taken at descending pressures to 1000 atmospheres as well. In all cases there appeared to be little or no hysteresis in the curves obtained.
This fact, as well as the fact that the exciton peaks sharpened at lower temperatures, -;;as especially encouraging since there was some concern about strains introduced both through differential therinal contraction and pressure induced strains. A further check was aade to determine the influence of the differential contraction of the sample and substrate.
The table below displays the results of evaporating TlCl onto various substrates.
Table 2. Comparison of pressure shifts of the exciton peaks in TlCl filiûs evaporated onto various substrates Substrate Coefficient of linear Pressure shift of expp.n.'iion (Û') x exciton peak x 10-u r /n TlCl ifeCl 40% -13.8 Fused quartz O.5G -14.1 SanDhire window 52 -7.8 ^•Rooin temperature values. takun at liquid niti-o/jon tonporabure. ^Reference 11. ^-Reference 12. Variations in film thickness from ^00 A to ilOOO A affected the pressure shift by only about 10/a for any given exciton peak studied. Thus the differences shovm in the shifts are thought to be due mainly to the various decrees of adhesion of the sample to the substr&tc. Althou.^h the fused quartz has a thermal expansion coeffi cient over two orders of magnitude different from that of TlCl, the measured pressure shift is only about lOJil different from the value obtained with a NaGl substrate, which has a thermal expansion coefficient similar to that of TlCl. The
TlCl film apparently adhered rather well to the sapphire, which lowered the pressure shift by a factor of two. All values of the exciton pressure shifts later reported will be from films on quartz substrates.
Previous work here by Mr, H. Sealock indicated "that AgCl films evaporated onto NaCl and Li? substrates exhibited exciton bands which broadened greatly upon cooling to liquid nitrogen temperature. This broadening was attributed to strains caused by differential contraction between the sample and substrate. The exciton bands in the films studied in this experiment all sharpened upon cooling, further evidence that the films adhered rather poorly to the substrates.
Since cooling 300 Kelvin degrees ca.uses about the same amount of strain from differential contraction as applying
3500 atmospheres of pressure causes strain from differential compressibility, a broadening of tha exciton peaks with increased,pressure would be expected if the film adhered well
to the substrate. Zallen (I5) found this to be true for pure silver films evaporated onto ouartz and sapphire compared to an unsupported silver file, as evidenced by greatly varying
pressure shifts of the peaks in transmission of the films.
Some broadening of the exciton peaks generally did occur in
the present experiment. Since the e:-:citon peaks are super
imposed on the absorption edjos, however s the fractional
change in height of the peaks could not accurately be deter mined, although it was clearly sznall. The extent of the dis
tortion introduced by differential compressibility of the
sample and substrate was felt to_oe. minor not only because
the broadening was slight, but also because the films did not adhere to the substrate as well as pure silver adheres to quartz. The spectra were measured on a Gary 14^ spoctrophotoMOter.
For all wavelengths greater than 3000 A a 65O watt accessory quartz-iodine lamp was used, 3alow 3OOO 2 the standard Gary hydrogen lamp v;as used. The spectra of both the exciton peak shifts and crystal edge shifts were taken at the fastest chart
speed (5 in./min.) and slowest wavelength drive (§A/sec) to
provide maximum accuracy in reading the data. The spectro
photometer was equipped with a 0 to 2 optical density (o.d.) slidewire, where r \ -^o 0.Û, =•• in -J- , 29
Iq being the reference bean intensity and I the sample beam intensity. , 0 Typical resolution for the thinner films v:as 4 A, and for o the thicker films about 10 A. In all cases for the absorption edge pressure and temperature shifts the resolution was better than 4 A. A calibration of the spectrophotometer in the o region of concern indicated that it was off only from ->1 A to '^4 A.
Due to the largo nusber of rsflectins surfaces (the cryostat windows, pressure cell windows, and sample) and the high refractive indices of the sapphire and the samples, as well as the greatly decreased beam dimensions in passing through the pressure cell, background optical densities of around one were common. To compensate for this neutral den sity screens were placed in the beam. The slit height was lowered to its minimum value (8 mm), and the slidewire balance control adjusted to yield a value near zero so that the full range of 0 to 2 o.d. units could be utilized. The background optical densities for the temperature measurements were some what lower, around 0.5 o.d. units, since the beam was not as constricted as when it passed through the pressure cell. The assembled cryostat, less sample, was placed in the usual con figuration on the spectrometer and a baseline run. This base line proved to be constant enough to neglect its effect on the spectra measured. 30
The temperature dependence of the absorption edge in TlCl and T'lBr vras measured from near liquid helium temperature to near dry ice temperature. The samples ^ere precooled to liquid nitrogen temperature, A spectrum -fas run at this point for later comparison. The helium transfer was then made and sufficient exchange gas introduced into the sample chamber to bring the pressure to about 50 microns of H3. This approxi mate pressure was maintained throughout the experiment by removing or adding small amounts of gas as needed. This sub stantial amount of exchange gas provided rapid and even cool ing in the sample _chamber, insuring that the temperature read by the thermocouple, which i«-.s attached to the aluminum sampleholder near the sample, was representative of the sample temperature.
A few minutes were usually allowed at each temperature for an equilibrium to be established. The heater was used to brins the sampleholder and sample to successively higher tem peratures. When moderate heat had to be introduced this way, more exchange gas was removed and the heat input reduced to obtain better temperature uniformity. After the nitrogen had boiled away in the inner reservoir this method could be used to raise the sample temperature to over 200*^K with consider ably less than 1 watt input» Again the spectrophotometer was run to obtain the 'maximum readout accuracy. 31
Fressure Dependence of Single Crystal Absorption Edges
Figure 6 displays the results obtained when the absorp tion edge of a AgBr crystal was maasurad at 10°K. The crosses represent data taken at 2100 atmospheres, while the circles represent data taken at zero atmospheres. The points at the extreme lower left of Figure 6 were obtained fron the data by finding the point where the slope of the edge leveled off.
This Was easily found directly froa the strip chart recording.
For ordinates greater than 1.^, the points lie on a straight line which connects them to the respective zero ordinate points when extrapolated. The portions of the spectra above these extrapolated lines are redrawn along the baseline of the graph. Notice that the area above the extrapolated straight line seens to be greater at the higher pressure. The hori zontal distance between the two straight lines gives the pressure shift of the onset of the crystal's absorption edge,
-1,9x10"^ eV/atm. The negative sign indicates a shift to lower energy with increasing pressure. The baseline zero was taken at the point where the o.d. due l;o thr- ah.-iorption re],\'r- rinnr.'M'rd to né;:rly I'^vd r/fr.
i.lKi ;^pccl;.ri;!:i coiil.U L'icii. uo ;;lope (in 'i. tc /•^î.v./i.ually toward longer wavelengths, this method of fixing the zero of the baseline introduced little or no error in the results. This conclusion was reached after the pressure shifts foand 2.0
2.70 275 2.80
INCIDENT PI :0T0N ENERGY K cV
Pisure 6. Absorption ecl^o of a A^Br single ory.otal at lO^K at 2100 aty. (x) and 0 atrn (o) 33
by plotuin;.'," the data In t;ho above rnnnnor v/orr; compared v,o those plotted using the mlnirnura value of the o.d., reachod near 0.6 microns as a baseline, as '/rell as those y ho so base lines v:ere shifted an arbitrary acioun'c as a test of the correctness of the procedure.
The data in Figure ? display the shape of "che A^Cl absorption edge at I83O atmospheres (crosses) and zero a"i:ao3- pheres (circles). The pressure shift of onset of the ed\';o was found to be eV/atZii. This value was usud since the curves tend to Berge at higher absorption» indicating that some competing absorption processes iray be occurring.
The points at the zero ordinate were again easily obtained.
Notice that here rather than an enhancement of the edge over a straight line extrapolated fron higher o.d., there is a marked dropoff near the beginning of the absorption edge.
The data in Figures 0 and ? trero scaled to compare %ith those of Bro:>m (14^1$) who has studied extensively the optica absorption of these salts. Brown plotted curves obtained fro the spectra of several crystals of vridely varied thicknesses, so that the present data correspond to only the lower values of (^hV )^' which he plots. The spectrum for the AgBr absorp tion edge from Brovm (14, Figure 8, p. 2372) and the spectrum from the present work (Figure 6, 0 atmospheres) vrere compared graphically. The values obtained for the onset of the a o *oJ 0.8
3.26 ;NT photon ENERGY IN cV
Figure 7, Absorption of a AgCl single crj'stal at 10°K at 1530 atr (X) end 0 ;r. (o) 35 absorption edge vrere 2.690 eV and 2.633 eV respectively.
This difference of 0.0C2 eV was the caximua discrepancy between the two spectra at any point.
When the curve in Figure 7 (0 atmospheres) was compared to those of Brown (14, Figure 9. p. 2373) for the AgCl absorp tion edge, they were found to possess the same general shape and slope. Although the curve from this work lay generally 0.004 oV to lower energies than Brown's curve at 4u2°K, part of this siiall discrepancy is attributable to the higher tu:.:- perature of the sample in this experiment (10°K). Llco 2rown detected at optical densities less than 0.01 a nearly hori zontal foot extending about 0.005 eV to lower energy on the absorption edge. This was not seen in this work because of the very small absorption level as well as the soaewhat poorer resolution than 3ro%m had. The two spectra for TlBr (Figure 8) appear more like those for Ag3r than those for AgCl. The crosses represent data taken at I89O atmospheres ; the circles represent data taken at zero atmospheres. The value of the pressure shift of the onset of the absorption edge was found to be -18x10"*° eV/ata. Again this value was taken at the onset of the steep absorption conponent. The curves again tend to vierge at higher o.d. Notice that the enhancement found here is of the general shape of that found for Ag3r, but srcaller. Also it is not clear that one curve is i:ore greatly enhanced than the other. 2.0
2.62 2 65 2.70
INCIDENT PHOTON ENERGY IN c\ Pigur-G 8. Absorption edge of a TlBr single crystp! c: lO^K at 1890 e.t-j (x) and 0 atrri ( o ) 37
Figure 9 gives the absorption edges for a single crystal
of TlCl at 1970 atmospheres and zero atmospheres. The value
of the pressure shift of the absorption edge as measured at
the onset of absorption is -16x10"^ eV/atm, Again the curves
tend to merge at higher o.d. The shoulders near the beginning
of the edges do not appear to be similar to those in TlBr and
AgBr. A straight line extrapolation from high o.d. falls far
to the high energy side of the horizontal intercept of the
curves, rather than nearly through the data points at the
In Figure 10 a comparison of the edges of the four single
crystal samples is made. The plots are the zero atmosphere
runs of the four preceding figures whose horizontal intercepts
have been shifted such that all the absorption edges begin at
the incident photon energy EQ. The ordinate could have been
expressed equivalently in terms of the absorption coefficient,
since the crystals all were of comparable thicknesses. In
that case the equivalent values of would range from zero to about 10 cm-1.
The ordinate plotted for the above figures, (o,d, x
hV )®, is equivalent to (ahy)® since the reflectivities
of the samples used here are small. Plots of the incident
photon energy vs. (o.d. x hV)^ (o.d. x hV")^/3, (o.d. x
hV), and (o.d.) were made to determine the best functional
dependence for the experimental points. These plots have been PHOIO.'J ENCRCY
Absorption edge of a YlCl sj.nslc or.vstr:! st Io"k at I97O ct;v-i (x) and 0 atra (o) 2.0
Tl Cl Tl B;
>C X) o s 0.0
E E^-!- 0.50
INCIDENT PHOTON ENERGY IN eV Picture 10. Cc nTgrlson of the absorption of A^Dr, A^Cl. TlBr, TICi 40
susiSested by other theories (lo, p. 202). Another poscibiiity for the functional dependence of the ordinate was suggested by
Urbach (1?). According to Urbach's rule, the optical absorp
tion increases exponentially 7:ith energy near the absorption
edge. The data conprisins Figures 6 through 10 were plotted
in this manner and fit a straight line well. In addition, the values of the pressure shifts obtained from the Urbach rule-
plots agree quite closely with those plotted using (o.d. 3: X. h"r)~ as the ordinate. Only the Urbach rule plot and the
(o.t'i. >: h^r )'• plot, dlrl noi". dcvlatr f from a
?rc^::3ure Dependence of Exclton Pea A:.; in Thin porabcd Kilnu"
The pressure shifts of the tvro observed oxciton peaks in
Ag3r are shcizn in Figure 11. The peak labeled A lies at about
2600 -? and appears as an unresolved huzp in the absorption
spectra of very thin films. Peak 3 is found at about 2900 a. The spectra were measured at liquid nitrogen temperature. The
peak position was arrived at by graphically determining the IVJLV. of the peak for at least two, and usually three,
traces of the region including the peak for each pressure attained. A least squares fi"c was not used since the number
of experimental points was sirall and fell nearly on a straight
line. A visual best fit Method provided anple accuracy. In
this and the following thin filzs; the films of each of the o four types studied whose thickness was most near 1000 i-. were 41
SL0PE = 3.4 :: eV/oim
Pisure 11. Typical pressure cf exciton recks in Agar thin filins
J used as examples of the results.
The slope in Figure 12 gives the pressure shift of the; exciton peak in a typical A%C1 film studied. Figure 13 dis
plays a typical run from a TlBr thin file» while the pressure shifû of the ezciton pea:-: in a TlCl chin fila is sho;/n in
Figure 14. Notice the large negative slopes in Pi.^^ures 13 and 14 compared with the sr^ller, positive slopes in Figures 11 and 12.
Temperature Dependence of the lixclton Peak Position
in Thin Films of TlBr and ?1C1
Figure 15 displays the temperature dependence of the exciton peak in a I36O A filra of T13r, The ordinate repre sents the energy of the exciton peak, obtained in the sar.e rianner as described for the exciton peak pressure shifts.
Notice that the slope changes sign at about 55°i'-. Figure I6 sho^s a typical temperature dependence curve for the exciton peak in a thin film of TlCl, Here the change of slops occurs at about 160°K. It is apparent in both of the above fiisures that neither curve can be fitted to a straight line at tem peratures below 300°K; however it seens reasonable to place an upper lisiit for the value of the slope of both curves near rooa temperature as 1x10"^ eV/^K.
The temperature dependence of a point near the onset of the absorption edge for single crystals of both T13r and TlCl v:as also measured. These curves were of the saice general 5.1 O'D >o
I?. L'J O O :c ii.
lU o o
O 1000 2000 3000 PRESSURE IN ATf/:0Sf'H[:RES i'in-urs 12. Typicr.l prespuro shift of thn obficvvecl. crciton pcr-.lc in ArCl tiiln filvris \
3 .06 - >- Ci) SL0PE^-:3.R3X!0 cV/a!m LU W 3 .05 -t- § % S 04
z hi S d 5 .03
1000 3 000 PRESSURE ID AT:.;0SPr!ER2S
Figure 13» Typical T>ressu:-v-. shift of the oba rvcd exciton peak in TlHr thin fil:i,H 0 eV/a
PRESSUuE IN AT|..10SPI:u\ES
Figure l/l'. Typical pressure shift of the observed ox ci ton peak in T'lC'l thin fillss l'Er.::''2RATURc, -"K
FiGUTc 15. Temperature dependence of the er'citon ],cak In a TlBr tlrln
shape as those obtained for- the exciton peak uemperature
shifts, but tended to have minima at lo^Yer teaperatures than
the curves displayed in Figures 15 and lo. At temperatures around 200°K these curves both h.v.d slopes of 3.7x10"^ &V/G%.
For reasons that will be mentioned later these curves are not
useful In Interpreting; the data and arc not displayed. ïh.^ data displayed in Figure 1? v.'ore obtained as follo'./:;. The upper noints, near absorption coefficients of 10^
were obtained from the spectrophotometer curves of the exciton peaks of the four salts at the time their pressure shifts vrere measured. These data were then corrected for the larrre back ground absorption caused by the pressure cell and cryostat.
The approicinate absorption coefficient could then be calcu
lated knowing the film thickness. Any increase in the reflec
tivity xrith decreasing wavelengths :7culd shift the points
obtained for the absorption coefficient of the thin filns to
slightly lovrer values. The peak positions vere corrected to
one atmosphere values « and plotted. The lower points are fron
single crystals, whose thicknesses were approximately 2 ion.
It has been found that Urbach"s rule is obeyed for several
orders of magnitude in_the absorption edges of cany crystals
(1, p. 128). Assuning that this is true here, the lo%er and
upper points could be connected by a straight line on a
logarithmic plot. Clearly this is not the case for AgCl,
I'.'here the two points to the extreme upper left of the graph rlcuie 17. Approzlraate absorption coefficients of crystals (Icire points) r.iicl thill filinw (upper pointe) for the four lifcj.iclc;-; stud ic;d APPROXIMATE ABSORPTION COEFFICIENT (mnf)
n o H
0Ç 51 are more than 0.1 eV froz a line extrapolated fron the single crystal data.
The temperature depcndcnce of the exciton peaks in A.~3r and A3CI thin filnis was not rxasurcd sinca the nature of tha transitions which give rise to then is «ell known, unlike the situation for the thallium halide excitons. 52
Table 3 summarizes the findinss cf the present work.
Negative signs indicate a shift to lower energy with an in
crease in pressure or temperature^ Broim (lA'O demonstrated that the absorption edge in AcjBr and AgCi is indirect. Bassani et. have pointed out that
the sharp absorption peak at about 5 eV in A3CI thin fil;"s is
most consistently associated with the direct exciton transi
tion from -che center of the Sr.:11 ou in zone. Referring to Figure 1?, it ic seen that for A.^Cl an
Urbach plot of the absorption coefficients for single crys
tals and thin films cannot be connected by a straight line.
The location of the sxciton peak is far to the left of the line extrapolated from the single crystal data. Although the effect in AgEr is far less striking, it can be seen that here
too this simple plot indicates that the single crystal absorp
tion coefficient seems to be rising above the straight line joining these points to the thin film absorption coefficients.
Since these lower points are known quite accurately, this deviation is real, even though scall, These are indications
that the excitons seen in the thin films are not related zo
"Che absorption edges se^n in the single crystals. A descrip
tion of such a system was made in the introduction using the well known example of germanium* The pressure shifts of the edge (Table 3» row 1) and of Table 3^ of pressure and temperature dependence data and calculated exciton bindinr;; cnor:^) rn Saiiple î'iearurf:)ront . ^?Br /'• .~C1 TlBr- TlCl
Pressure shift of absorption edge, in units of 10-^ eV/stT,i. -1.9 -1.5 -lo -.1&
Pressure shift of exci ton poalc, G^k- in units of 3.0'-^ eV/atni. 5«6 6.2 -'IJ.h -13.9
Tenperatn.re shift of absorption cdo-e, ^ positive^ positive^ in units of lO-^!- cV/°K =7.8^ -8.7^- 3065 3.67
Temperature shift of exci ton peo.]:, positive" positive^ in units of 10--^^ eV/'^K -•» --- 1 1
Pressure shift of the r^ap enoi'sy, ^ vn in units of 10- - oV/ati...^ 4.6^ -15.6^
Calculated binding energy of ezciton usins' r.'annicr inodr;!, in eV _ 0„0'!y 0.065Ç ^ _ 0t07^%
^Values t^lzcn fron' ?j sure s 6 and 7, Reference 1': .
^Slopo determined near rooa temperature.
^'Tbis quantity is detornined by s^Jbtractinj; an estimate of the pressure dependence of the ozciton binding ener/gy from the observed exciton peak pressure shift.
ef er e n c c 1 8,
^Reference ] ,
^fieferenoe 20, the exciton peaks (rovr 2) of the silver salts have opposite signs, indicating that the quantities measured are no'c repre senting the sane type of transitions (3). Assuming the exciton is a cannier exciton, chu oqii..,wion
1 Rydbera B(p) [Gs(p)]2 a inay be used to calculate the pressure dependence of the exciton binding energy. The value of is taken as 1/2, although this value say be less than 1/2 for direct excitons
(Brc:-m 14). The static dielectric constant, has been used in the denominator. The assurjpticn that '.vannier excitons are involved is nost valid for the case of indirect excitons, but na;r also be applied to direct excitons. In either case it is at worst an under estizzzate of the exciton binding energy. using the values of recently measured by Jones (19) it vras. found that the pressure shift of the gap associated >rith the exciton in AgCl, found by subtracting the pressure dependence of the exciton binding energy, 3(p), frca the measured exciton peak pressure shlfu., was reduced by 23 per cent (row 6). This still preserved ohe original opposite sign relationship between the pressure shifu of the absorp tion edge and that of the exciton. This is further proof that the absorption edge and the edge associated with the exciton are not the same. No data for the pressure depend 55
ence of the dielectric const&ns of A,g3r are available, baô it
is assumed that, since the dielectric constant for Ag3r is
similar to the value for A3CI, the outcome of subtracting
B(p) from the zeasurad exciton pressure shift vrould be similar
to the results obtained for A3CI. The data in Figure 6 may be interpreted as follows. The
onset of the indirect absorption edge is at (3^ - 5 j: kG).
The enhancement of the edge due to the electron -hole coulonb
interaction oxtcvifi;: to titi'ihr':- th.-m fiu-i onxrt oV tti:-
uu; by ::i;Vcr,'.1 Lliiu;;; I:, i;lu; u:::0,1 iij.iuUiK': (jucr:'.y\ Tiic region of enhancement of the absorption rrill be pressure de
pendent. From Jones' (19) work it is knov;n that the dielec
tric constant decreases vrith increasing pressure. Assuming a
Wannier exciton, B(p) is proportional to G-2\ This o-eans that T:he exciton binding energy increases with increasing r^ressure.
Pot the prer;euro ran-jo .%ivcrt ir, l''i,;i:re 6, this lnoroa;>'; v;o.;là
ht; nboxt '/,v. 'I'hc; rtxl incrcanf: 01' tho cncr/ry ran; '.vhcrc the absorption is enhanced is about 'K.'. The A^Cl absorption ed.-jos displayed in Figure 7 do not
exhibit the same enhancenent that the A^Br curves exhibit. The reason for this likely involves the complexity of the AgCl edge compared to the AgBr edge. 2ro;-.n (14) has observed
four hus^s near the onset of "che absorption edge in AgCl,
generally only 0.02 to 0.03 2V apart fron each other. Eassani
at al. (4) feel that these are due to various L-type and 2- 56 type transitions. Each of these transitions "'rould have o. spectrum similar to ths.t seen in the AgBr edge, but a co::- bination of the four spectra, displaced only a few hundredths of an eV apart from one another could produce an edge irhich looks like those in Figure 7» The data for the thallium salts are also enlightening.
The larse negative pressure shifts of the absorption edces are about equalled by the- large negative pressure shifts of the vjxciton peaks. It Ik reasonable to conclude from thl;; inforiiiation ch.it the antiorption nr:a;;\'r(:d in oho u l/ixlc crystals is the low absorption coefficient tail of the ezciton band seen in the thin films.
When corrections are applied for the pressure depend ence of the exciton binding energy, using the wannisr model again, the effect is to increase the observed exciton peak pressure shifts so that they nearly coincide ••rith the corres ponding values for the absorption edge shifts. The assumption that the VJannier e::citon sodel can be used here is even ^ore justifiable than its use for the silver salts, since "ohe dielectric constants for the thallium salts are huge. That the pressure shifts for the pressure dependence of the band gap corresponded liore closely to the shift of the onset of the absorption edge for both thallium halides is probably a coincidence» It is likely that pressure affects the halfv/idth of the exciton band slightly, so that a point 57 many halfwidth distances below the peak, namely near the onset of the absorption edge in single crystals, would be likely to have a slightly different pressure shift than the exciton peak.
The conclusion that the edge seen in single crystals is simply the low absorption coefficient tail of the exciton band seen in thin films is further borne out by the data in
Figure 1?, For both TlBr and TlCl the lower and upper sets of points are joined well by a straight line, indicating that, if Urbach's rule is obeyed, they arise from the same transi tion.
The slope of the absorption edge shifts rapidly with increasing temperature, but much of this shift is due to the broadening of the edge as the energy bands become thermally blurred. The shift of the edges in TlBr and TlCl was taken from the shift of points at an optical density of unity after subtracting the background absorption. This was done not only to compensate somewhat for the above effect, but also because the onset of absorption became increasingly difficult to ascertain as the temperature rose. A similar effect occurs for the exciton peak temperature shift, but is smaller in magnitude.
Zinngrebe (21) has carefully studied this effect in TlCl.
He found that at temperatures above 150°K, the onset of the absorption edge shifts rapidly to longer wavelengths, while 53
the exciton "band peak as measured in thin filais shifts to th's
red at a much slower rate. Thus the exciton peak shift is
less of an overestinate of the intrinsic ed^e shift with teo.-
perature than the shift at or near the onset of the absorption
edge. Because of this effect, little value vras attached to the measurements of the temperature shifts of the absorption edges in the single crystal samples. The temperature shifts of the exciton peaks in TlCl and
T13r sho%^d unusual slope reversals (ssc Figures 15 and 16), as did the curves obtained froia the single crystal temperature dependences, but at higher temperatures. The slope above this
minimus in each case was not linear, unlike the data obtained for the single crystals. 3y subtracting the temperature de pendence of the cxciton binding energy calculated from the values cf e(T) obtained by Saraara (IS), the ninisa of the curves tended to shift to even higher energies, since 3(T) was a nionotonically decreasing function which raised the value cf the lor: temperature negative slopes and lowered the values of the high temperature positive slopes. Thus the curves for the te&perature dependence cf the energy gaps asso
ciated with the excitons in T13r and TlCl would appear to be rotated counterclockwise with respect to those for the tem
perature dependence of the exciton peaks alone and also shifted to higher energies by the amounts of %he exciton binding energies, which appear in Table 3, row 6. 59
This procedure did not yield a straight line fit for the
high temperature slope, ho'-rever. Plots of the data "bsfore
subtracting the temperature-dependent exciton binding energy,
using various ordinates and abscissas, vrere likevxise unsuc
cessful in giving a straight line slope at high temperatures.
The values of ^IxlC"^ eV/°K quoted for the exciton peak zez-
perature shift for each thallium salt are felt i;o represent
the upper limit of the excitcn shift, and were determined at
the highest temperature laterv^ls r^asurcd to obtain "J.he high est slope values. If the cxclton and the absorption edge
represent transitions involving the sase direct edge, as is
suggested by the data, this value also represents the upper Unit of the intrinsic absorption edge shift as measured at
high temperatures. Zinngrcbe (21) has suggested that the much
creator t.-^np.ii'atnrr nhift of th>"> In ihi<; to hlviirr tcuipcr- aburc transi tiorvi; occurrln,/ near Lhc foot of the ab:;orntion
edge. The temperature dependence and pressure shifts of the absorption edges and e::ci ton peaks can be used to determine
the quantity (oE/oT)y using
/aE', f23\ IS?;, = •
Here K is the Isothernal cornpressibllity and %' the volume isobarlc thermal expansion coefficient. Thus the temperature shift can be broken into a portion due to thermal expansion 6o alone, -3&/K(oE/oP)^, and a portion due to lattice vibration effects, OE/ôT)y. Since the absorption ed^e and excitons are optical manifestations of the crystal as a v.-hole.j the bulk values of <% and K should be appropriate. The tenperat-ire shifts are taken at or near room temperature, and the value of (3E/3p)^ at 80°K is assumed to be the same or only slightly smaller than its value at roora temperature. Table sur.;r.ar- izes the results of substitution into this equation. Notice that in every case (3Z/6T)y ic negative, as expected (2^:).
Piû'ure 13 displays the tv.-o available calculations for the band structure of Ag3r. These band structures are the results of two calculations, each utilizing a different method and potential function. Bassani et al. (4) used a tight-binding method. The valence band structure -vas calculated, while the conduction band shape vas es tir,at ed to best fit the existing data, ocop ( 5) carried out av; l;ecl plnno wave calcula tion to obtain both the valence and conduction bands. Ho adjusted the hand structure to fit the experimental valiu-s of the direct gaps at the center of the 3rillcuin zones in each crystal. Only the uppermost valence band and the lovrest con duction band fros: these calculations are sho'm here. The energy bands for other crystal syaaetry directions vrere also
Given by Scop, but only the directions of highest syanetry, hence of hi^hnst density of states, have been shoivn. The li_(iiO) dlroctionj levels have been inaic.:itud by the linos Table Calculation of (ôE/ôT)y for the four halldes studied, using the equation ÔS\ _ fôE\ 3» /ÔEN ôT/p - Ut/V " K lap/?
Crystal 3VK (âE/aP)T 3*/K(aE/ap)T (aE/aT)p (aE/aT)v atm/°K xlC^eV/attn xlO-4 eV/OlC xlO-4 eV/OK xlQ-^ eV/OK
AgBr^ 44.5b -1.5° -0.67 -7.8° -8.5
AgCl* 39.2 -1.9° -0.74 -8.7* -9.5 TlBr& 34.0® -15.8^ -5.37 1^ -4,4 to -5.4 T1C1& 37.0® -16.yf -6.18 if -5.2 to -6.2
Indirect absorption edge. ^Calculated from values of C^it and Czj.z(, from Reference 23. ^Reference l4. *^Direct absorption edge. ^Reference 11, ^Data from Table 3. 62
2.80 eV 4.2S eV cc 1 (h.h.o)
-4L I •(h,h,h) (o,o,o) (o.ovh)' L L r A X WAVELENGTH ALONG SYivl ŒTÂY DIRECTIONS
Ef.nd structure calculations for AgSr, .fJï £ii» (solid iir.es) and Scop (5) (dashed lines) 63 to the right of the main band structure diagram. The t-./o conduction band miniroa were superimposed graphically zo have a coamon minimum, while the valence bands vrere adjusted as follows. The indirect edge (1^,- to / ^) was adjusted to fit the experimental value (2.80 eV) for Eassanl's bands, whereas the direct edge transition (Pt^ to ) was made to fit the experimental value (4.29 eV, as given by Scop) for Scop's bands. This was in keeping with the original adjusting
oT ti'xrxinnl ari'i C-cop. , \ roupondlng to Ibcuani's band juructurc, while the dashed lines are those of Scop's calculations.
Table 5 contains the energies for direct transitions froia the various valence band naxlina to the conduction band. These figures are only approximate, and are siven in the notation used by Bassani.
Table 5. Snersies of the direct transitions frca the valence band roaxima in A~3r
Transition Bassani, et ai. (4) Scop (5)
ri5 to p 1 4.5 eV 4.29 eV
A^toA^ 4.'7^ eV
to ^2 6.15 eV 6.0 eV
to 6.0 eV 64
Figure 19 displays the corresponding band structura for
AgCl. The same description as for Figure 18 applies, except that the indirect transition, thought to correspond to the indirect absorption edge (L^ to p has an energy of 3.22 eV
(4), while the direct transition at the Brillouin zona center has the value 5.13 eV (5). Table 6 is a sunroary of the direct transition energies from the various valence band roaxiica in
Tabic 6, EnsrgiGs of the direct transitions frou the valenco band riaxiiiia in Af;Cl
Tran sition Bassani et al. (4) Scop (5)
. r! to cM 5.11 oV 115 T'l 5.'I-5 to Ai 4.40 eV 5.70 eV - » to 6.30 eV 7.10 eV -"3 ^2
-4 to -1 " 0 .(>')
Sketches of the absorption edges of thin filras of AgBr and A3CI appear in Figure 20. The energies of the transitions from Tables 5 and 6 are shovn.i as solid arrovrs (Bassani) and dashed arrows (Scop). Looking at Figure 20a, ue sea that the two values of i ' ]_5 cuiï;e near the hi^h energy valley asso ciated vrith the first e::ci ton peak seen. If this exciton is due to a direct transition, it should appear at 3^ - 3. Thus the distance fron the valley to the peak represents the exciton binding energy, while the energy of the gap related to the 65
WAVELENGTH ALONG SY[, Band structure •^1. (4) (solid lines) Eg 2.0 3.0 AgCI
>- > t- CO 1330 A FILL'. (/} l'j Q Q
-1 .! O I- D„ O LU l.'l 750 A FIL I-
c>>< g 2.0 n: CL. ù. D., o. < <
.20 .50 5 4 28
V/AYELKNGTH IN (/ICROiJS
Figure 20. Location of calculated transitions on roctions cf the AcBr and ArrCl t-hivi il In cbsorjition edges 6? exciton is Eg, The transition A5 points to a hump in the
structure of the thin film which is resolved in the thicker film. Because of the location of the A5 transition on the energy band structure, it should appear as a weak peak at
best, since the density of states is low. Probably this hump is due to spin orbit splitting of the direct P transition, which was not included in either band structure calculation.
The small arrows to the left of the exciton peaks in Pig^are
20 represent the position of the direct edge energy gaps cal culated by subtracting the exciton binding energies from the measured exciton peak positions, assuming Wannier excitons are involved with effective masses of 0.5- These energies are tabulated in Table 3» row 6. That the arrows indicating the transitions in Figure 20 do not all coincide nor all point to logical positions for an energy gap location is an indication of the uncertainty in the band structure calculations.
It is not clear what dielectric constants should be used to calculate the direct exciton binding energy. Values of the optical dielectric constant (14), the static dielectric constant^, and some intermediate value between these (24) have been suggested. The values used here are for the static di electric constants, which give at worst an underestimate of the exciton binding energy,
^Lynch, D. W,, Ames, Iowa. Data from P, C. Broim, Urbana, Illinois, University of Illinois, Physics Department, Private communication, I967, 68
The spectrum in Figure 20b represents the absorption edge of a thin film of AgCl near the exciton peak. The two energies calculated for the P 15 to P" transition straddle the experimental location, for the direct gap energy. Again the binding energy was estimated using a Wannier model exci ton. Both here and for the two exciton peaks in the AgBr film, this value falls short of the experimental value which may be estimated from the energy which separates the exciton peak from the high energy valley nearby. The extent of this discrepancy is an indication of the degree to which the excitons involved are different from ideal Wannier excitons. Sketches of the portions of the absorption edges near the exciton peaks in TlBr and TlCl are given in Figures 21a and 21b, respectively. Assuming that the excitons are direct
Wannier excitons, the energy gaps have been calculated (Table
3, row 6). These appear as arrows pointing to the short wave length valleys associated with the exciton peaks. The agree ment of the calculated energy gaps and the measured gaps is excellent, indicating that the Wannier model described these excitons well. This is in agreement with the assumptions made in the Wannier model, since the dielectric constants of TlBr and TlCl are very high.
The results of Slykhouse and Drickamer (25) and Zahner and Drickamer (26) may be interpreted in the light of the data taken in this work. Slykhouse and Drickamer measured the TIBr
Figure 21, i.oc;'i.ion of c-lculatcd TlCl thin filîn abfjcrutj 70
pressure shift of the absorption ed^s in the silver halides
to very high pressures. In the pressure ranse used in -.lis
woi-k, their values for the edge shifts were -3%10~? eV/&tz and -bxlO~7 eV/atn for AcBr and AcCl respsctively. These
values are both only a fraction of the values of the shifts observed in this work at the onset of the absorption ed'je, but this can be readily explained since their msasurements v:ers not made at the onset of the ed^a. Tiie farther a^ay frcni the
onset of the absorption adjs Koanr.rczenuS are r;„vlci, the
more effect the pressure shift of the airect ed^e, which is of opposite sign, will have on the net pressure shift of the ed.se. 71
SUMMRY AND CONCLUSIONS
The silver halide absorption edges have been extensively studied, and it has been generally accepted that for both AgBr and AgCl, the edge seen in the single crystals is indirect, with direct excitonic transitions apparent in thin film spec tra superimposed upon this indirect edge. The band structure calculations have not been able to determine which of the several valence band maxima are responsible for these indirect transitions. Bassani et sA. (4) suggested that either the to n or the to P 2.S transition could account for these spectra, while Scop (5) indicated that the transition is the
to P2.$' From the results of this work, it can be con cluded that whichever valence band maximum is involved, it is likely the same for both AgBr and AgCl. This conclusion is reached when the implications arising from the nearly identi cal pressure shifts of the indirect absorption edges in the two halides are considered. The complicated band structure for these halides arises from the overlapping of the many silver p and halogen d states. Since the symmetry properties at 2 and L are quite different, one would expect much differ ent pressure dependences of transitions originating from these points to result (3). Since this is not so, the transitions are thought to arise from the same symmetry locations in both AgBr and AgCl.
Using ultrasonic excitation of uniaxial strain, Ascarelli 72
(2?) has found that the valence band maximum in the (111) direction (L-symmetry) is responsible for the indirect trans ition in AgBr. Thus from the above argument, it may be asserted that the L to P transition is responsible for the indirect absorption edge in both AgBr and AgCl, Knox (28) has pointed out that the 5 eV excitonic transi tion in AgCl is anomalous, since a spin-orbit splitting of at least 0.1 eV is expected, while a splitting of only 0.05 eV is observed. For AgBr, the spin-orbit splitting is observed to be about 0.6 eV, which is close to the expected value. This o ,0 appears as the two peaks at 2900 A and 2o00 A in Figure 20a, which have understandably nearly the same pressure shifts as measured in this work.
The results for the thallium halides are quite consistent.
They all imply a direct edge which is the low absorption co efficient tail of the direct exciton band seen in the thin films. These results are consistent with the findings of îîakita et a2. (29) who have determined from magnetoresistance measurements that the valence band in TlCl is spherical and located at zero wave vector. Tamura and Masumi (30) and Hodby et (24) have measured the cyclotron resonance of TlCl single crystals and found that these measurements indicate a simple conduction band with its minimum at zero wave vector.
Further indication that the exciton peak and the absorption edge seen in single crystals are manifestations of the same, ?3 direct transition in the thaliiura h.:.iid.es is the similarity their temperature clependsnoaG.
Fro% Table 4 we see that the valus of (oE/6T)y for uho thallium halidcG is negative nnd choroforo nob nnoralou, even thou.'ih tho tompcraturo dependence of the abr:crpT:ion ed/; in these halides is anomalous. 74
. 1. Dexter, D. L. and R. S. Knox. Excitons, New York, New York, Interscience Publishers. 1965.
2. McLean, T. P. Excitons in Germanium. In Kuper, C. G. and G, D. Whitfield, eds, Polarons and Excitons, pp. 367-375» New York, New York, Plenum Press. I962, 3. Paul, William, Band Structure of the Intermetallic Semi conductors from Pressure Experiments. Journal of Applied Physics 32; 2082. I961. 4. Bassani, P., R. S. Knox, and W. Beall Fowler, Band Structure and Electronic Properties of AgCl and AgBr. Physical Review 137i A1217. 1965. 5. Scop, Peter M. Band Structure of Silver Chloride and Silver Bromide. Physical Review 139: A934. I965. 6. Brothers, A. D. The Effect of Pressure on P Center Luminescence. Unpublished M.S. thesis. Ames, Iowa, Library, Iowa State University. I965.
7. Bridgeman, P. W, The Physics of High Pressure. London, England, G. Bell and Sons, Ltd. 1949.
8. Pinnemore, D, K., J. E. Ostenson, and T. P. Stromberg. Secondary Thermometer for the 4 to 20®K Range. Review of Scientific Instruments 36: I369. 1965. 9. Heavens, 0. S. Optical Properties of Thin Solid Films. New York, New York, Dover Publications, Inc. I965. 10. Dugdale, J. S, The Equation of State of Solid Helium, Nouvo Cimento 9 Supplement 1; 27. 1958. 11. Ballard, Stanley S., Kathryn A. McCarthy, and William L. Wolfe, eds. Optical Materials for Infrared Instrumenta tion. Ann Arbor, Michigan, Physics Department, Univer sity of Michigan. 1959. 12. Hodgman, Charles D., ed. Handbook of Chemistry and Physics. Forty-First Edition. Cleveland, Ohio, Chemical Rubber Publishing Company, i960.
13. Zallen, R. The Effect of Pressure on Optical Properties of the Noble Metals. In F, Abeles, ed. Optical Proper ties and Electronic Structure of Metals and Alloys, 75
pp. 164-17^. Amsterdam, Netherlands, North-Holland Publishing Company, I966.
14. Brown, Frederick C. Electronic Properties and Band • Structure of the Silver Halides. Journal of Physical Chemistry 66; 2368. 1962. 15. Brovm, F. C., T. I'lasumi, and H. H. Tippins. Fine Struc ture in the Absorption Edge of the Silver Halides. Journal of the Physics and Chemistry of Solids 22: 101, 1961. 16. Smith, R. A. Semiconductors. Cambridge, England, Cambridge University Press. 1959.
17. Urbach, P, The Long Wavelength Edge of Photographic Sensitivity and of the Electronic Absorption of Solids, Physical Review 92: 1324. 1953. 18. Jones, B. V/, The Dielectric Constant of Ionic Solids and Its Change with Hydrostatic Pressure, Philosophical Kagazine I6: 1005. 1967. 19. Samara, G, A, Temperature and Pressure Dependence of the Dielectric Constants of the Thallous Halides, Physical Review I65: 959. I968,
20. Smith, G, C. Luminescence and Photoconductivity in Silver Halides, Unpublished Ph.D. thesis. Ithaca, New York, Library, Cornell University. 1965.
21. Zinngrebe, Horst, Die Optische Absorption von Thallium- chlorid, Zeltschrift fur Physlk 154; 495. 1959. 22. Pan, H, Y, Temperature Dependence of the Energy Gap In Semiconductors, Physical Review 82; 900, I95I. 23. Tannhauser, D, S,, L, J, Bonner, and A. W, Lawson. Tem perature Variation of the Elastic Constants of AgBr, Physical Review 102: 1276, 1956, 24. Kodby, J. W., J. A. Borders, P. C, Brown, and S, Poner, Cyclotron Resonance of the Polaron in KCl, KBr, KI, RbCl, AgCl, AgBr, and TlCl, Physical Review Letters 19: 952, 1967.
25. Slykhouse, T. S, and H. G, Drickamer, The Effect of Pressure on the Absorption Edge in Silver Halides, Journal of the Physics and Chemistry of Solids ?: 207. Zakner, J. C. and H. G. Drickacer. Tno Effect of pres sure on the Absorption lyi Heavy-1 let:.l Halidaz. Journal of the Physics and Chazistry of Solids 11: 5-. 1959. AsCc.relli, G. Ezpsrizsntal Dstection of Interne.! Polar Spates Associated tilth, the Indirect Zdjs of A^Br U^inj riezo-Oytical Transmission. Physical Review; Letters 20 44. 19680 Knox, R. S, and N. Inoha^spâ. E::ci ton States in Ionic Crystals. Physical Pievie'/: ll5: 1093. 1959» I'akita, ïunosuke, Koichi Kch-ycshi,, ;:.nd .lihoko ICanaca, Valence Band from the Transient hagnetoreeiscance of Koles in Ï1C1,, Journal of "cho Physical Society of Ja'oa 2]: 1180. 1967. Tarr.ura, Hiroshi and 'a..i3e l-;aeu.ai. Observation of Cyolo tron Resonance in TlCl. Journal of uhe Physical ScciOv of Jaran 2): 1173. 1967- 77
I vrish to express zy greatest appreciation to Dr. 3. V,'.
Lynch for his guidance in svery phasa of this :;crk, vithout which it -could not have lbs an possible to cccplete. 1-ly chunks go to Dr. R. %. riorgCLn for his assistance ^nd l-rnovrled^e in preparing the thin film samples, ?or the extremely pure samples of An;3r and A3CI I thank Dr. R. £. Van Hcyninjen. For advicr: on the design of the pressure eruip;uent and for the construction of the apparatus i thank Dr^ C. i. iv;c:-:son, :(r. Dean D„ Woods, and Kr, 2. nussell Clark;